The material structure described by NaLi5Mn2P2(CO7)2 crystallizes in the monoclinic P2_1 space group. Na(1) is bonded in a 7-coordinate geometry to one O(13), one O(14), one O(2), one O(3), one O(6), one O(7), and one O(9) atom. There are five inequivalent Li sites. In the first Li site, Li(1) is bonded in a 5-coordinate geometry to one O(1), one O(4), one O(5), one O(7), and one O(8) atom. In the second Li site, Li(2) is bonded in a 4-coordinate geometry to one O(10), one O(2), one O(3), and one O(9) atom. In the third Li site, Li(3) is bonded in a 5-coordinate geometry to one O(1), one O(11), one O(12), one O(5), and one O(9) atom. In the fourth Li site, Li(4) is bonded in a 5-coordinate geometry to one O(1), one O(10), one O(11), one O(12), and one O(5) atom. In the fifth Li site, Li(5) is bonded to one O(13), one O(14), one O(2), one O(6), and one O(8) atom to form distorted LiO5 trigonal bipyramids that share  a cornercorner with one P(1)O4 tetrahedra and corners with two equivalent P(2)O4 tetrahedra. There are two inequivalent Mn sites. In the first Mn site, Mn(1) is bonded in a 6-coordinate geometry to one O(11), one O(14), one O(3), one O(5), one O(7), and one O(8) atom. In the second Mn site, Mn(2) is bonded in a 6-coordinate geometry to one O(10), one O(12), one O(13), one O(4), one O(6), and one O(9) atom. There are two inequivalent C sites. In the first C site, C(1) is bonded in a trigonal planar geometry to one O(1), one O(3), and one O(5) atom. In the second C site, C(2) is bonded in a trigonal planar geometry to one O(2), one O(4), and one O(6) atom. There are two inequivalent P sites. In the first P site, P(1) is bonded to one O(11), one O(12), one O(7), and one O(8) atom to form PO4 tetrahedra that share  a cornercorner with one Li(5)O5 trigonal bipyramid. In the second P site, P(2) is bonded to one O(10), one O(13), one O(14), and one O(9) atom to form PO4 tetrahedra that share corners with two equivalent Li(5)O5 trigonal bipyramids. There are fourteen inequivalent O sites. In the first O site, O(1) is bonded to one Li(1), one Li(3), one Li(4), and one C(1) atom to form a mixture of edge and corner-sharing OLi3C tetrahedra. In the second O site, O(2) is bonded to one Na(1), one Li(2), one Li(5), and one C(2) atom to form distorted ONaLi2C tetrahedra that share  a cornercorner with one O(8)Li2MnP trigonal pyramid and  an edgeedge with one O(13)NaLiMnP tetrahedra. In the third O site, O(3) is bonded in a 2-coordinate geometry to one Na(1), one Li(2), one Mn(1), and one C(1) atom. In the fourth O site, O(4) is bonded in a distorted bent 120 degrees geometry to one Li(1), one Mn(2), and one C(2) atom. In the fifth O site, O(5) is bonded in a 5-coordinate geometry to one Li(1), one Li(3), one Li(4), one Mn(1), and one C(1) atom. In the sixth O site, O(6) is bonded in a 1-coordinate geometry to one Na(1), one Li(5), one Mn(2), and one C(2) atom. In the seventh O site, O(7) is bonded in a 4-coordinate geometry to one Na(1), one Li(1), one Mn(1), and one P(1) atom. In the eighth O site, O(8) is bonded to one Li(1), one Li(5), one Mn(1), and one P(1) atom to form distorted OLi2MnP trigonal pyramids that share  a cornercorner with one O(1)Li3C tetrahedra,  a cornercorner with one O(2)NaLi2C tetrahedra,  a cornercorner with one O(13)NaLiMnP tetrahedra, and corners with two equivalent O(11)Li2MnP tetrahedra. In the ninth O site, O(9) is bonded in a 4-coordinate geometry to one Na(1), one Li(2), one Li(3), one Mn(2), and one P(2) atom. In the tenth O site, O(10) is bonded in a 4-coordinate geometry to one Li(2), one Li(4), one Mn(2), and one P(2) atom. In the eleventh O site, O(11) is bonded to one Li(3), one Li(4), one Mn(1), and one P(1) atom to form OLi2MnP tetrahedra that share corners with two equivalent O(8)Li2MnP trigonal pyramids and  an edgeedge with one O(1)Li3C tetrahedra. In the twelfth O site, O(12) is bonded in a 4-coordinate geometry to one Li(3), one Li(4), one Mn(2), and one P(1) atom. In the thirteenth O site, O(13) is bonded to one Na(1), one Li(5), one Mn(2), and one P(2) atom to form distorted ONaLiMnP tetrahedra that share  a cornercorner with one O(8)Li2MnP trigonal pyramid and  an edgeedge with one O(2)NaLi2C tetrahedra. In the fourteenth O site, O(14) is bonded in a distorted rectangular see-saw-like geometry to one Na(1), one Li(5), one Mn(1), and one P(2) atom. is represented by the CIF card [CIF]
data_NaLi5Mn2P2(CO7)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   6.682
_cell_length_b   8.634
_cell_length_c   9.997
_cell_angle_alpha   87.605
_cell_angle_beta   90.000
_cell_angle_gamma   90.000
_symmetry_Int_Tables_number   1
_cell_volume   576.282
_cell_formula_units_Z   2
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Na  Na0  1  0.998  0.248  0.876  1.0
  Na  Na1  1  0.498  0.752  0.124  1.0
  Li  Li2  1  0.255  0.084  0.619  1.0
  Li  Li3  1  0.250  0.091  0.124  1.0
  Li  Li4  1  0.030  0.266  0.368  1.0
  Li  Li5  1  0.468  0.267  0.366  1.0
  Li  Li6  1  0.475  0.270  0.865  1.0
  Li  Li7  1  0.530  0.734  0.632  1.0
  Li  Li8  1  0.968  0.733  0.634  1.0
  Li  Li9  1  0.975  0.730  0.135  1.0
  Li  Li10  1  0.755  0.916  0.381  1.0
  Li  Li11  1  0.750  0.909  0.876  1.0
  Mn  Mn12  1  0.746  0.351  0.633  1.0
  Mn  Mn13  1  0.748  0.354  0.143  1.0
  Mn  Mn14  1  0.246  0.649  0.367  1.0
  Mn  Mn15  1  0.248  0.646  0.857  1.0
  P  P16  1  0.250  0.406  0.602  1.0
  P  P17  1  0.249  0.408  0.109  1.0
  P  P18  1  0.750  0.594  0.398  1.0
  P  P19  1  0.749  0.592  0.891  1.0
  C  C20  1  0.750  0.038  0.614  1.0
  C  C21  1  0.759  0.043  0.112  1.0
  C  C22  1  0.250  0.962  0.386  1.0
  C  C23  1  0.259  0.957  0.888  1.0
  O  O24  1  0.249  0.108  0.415  1.0
  O  O25  1  0.282  0.099  0.923  1.0
  O  O26  1  0.756  0.079  0.737  1.0
  O  O27  1  0.752  0.079  0.237  1.0
  O  O28  1  0.745  0.142  0.516  1.0
  O  O29  1  0.741  0.152  0.019  1.0
  O  O30  1  0.062  0.314  0.649  1.0
  O  O31  1  0.430  0.307  0.656  1.0
  O  O32  1  0.067  0.303  0.151  1.0
  O  O33  1  0.432  0.318  0.168  1.0
  O  O34  1  0.255  0.417  0.445  1.0
  O  O35  1  0.755  0.424  0.350  1.0
  O  O36  1  0.267  0.422  0.953  1.0
  O  O37  1  0.729  0.426  0.840  1.0
  O  O38  1  0.255  0.576  0.650  1.0
  O  O39  1  0.755  0.583  0.555  1.0
  O  O40  1  0.229  0.574  0.160  1.0
  O  O41  1  0.767  0.578  0.047  1.0
  O  O42  1  0.562  0.686  0.351  1.0
  O  O43  1  0.930  0.693  0.344  1.0
  O  O44  1  0.567  0.697  0.849  1.0
  O  O45  1  0.932  0.682  0.832  1.0
  O  O46  1  0.245  0.858  0.484  1.0
  O  O47  1  0.241  0.848  0.981  1.0
  O  O48  1  0.256  0.921  0.263  1.0
  O  O49  1  0.252  0.921  0.763  1.0
  O  O50  1  0.749  0.892  0.585  1.0
  O  O51  1  0.782  0.901  0.077  1.0
[/CIF]
.
The material structure described by NaLi5Mn2P2(CO7)2 crystallizes in the monoclinic P2_1 space group. Na(1) is bonded in a 7-coordinate geometry to one O(13), one O(14), one O(2), one O(3), one O(6), one O(7), and one O(9) atom. There are five inequivalent Li sites. In the first Li site, Li(1) is bonded in a 5-coordinate geometry to one O(1), one O(4), one O(5), one O(7), and one O(8) atom. In the second Li site, Li(2) is bonded in a 4-coordinate geometry to one O(10), one O(2), one O(3), and one O(9) atom. In the third Li site, Li(3) is bonded in a 5-coordinate geometry to one O(1), one O(11), one O(12), one O(5), and one O(9) atom. In the fourth Li site, Li(4) is bonded in a 5-coordinate geometry to one O(1), one O(10), one O(11), one O(12), and one O(5) atom. In the fifth Li site, Li(5) is bonded to one O(13), one O(14), one O(2), one O(6), and one O(8) atom to form distorted LiO5 trigonal bipyramids that share  a cornercorner with one P(1)O4 tetrahedra and corners with two equivalent P(2)O4 tetrahedra. There are two inequivalent Mn sites. In the first Mn site, Mn(1) is bonded in a 6-coordinate geometry to one O(11), one O(14), one O(3), one O(5), one O(7), and one O(8) atom. In the second Mn site, Mn(2) is bonded in a 6-coordinate geometry to one O(10), one O(12), one O(13), one O(4), one O(6), and one O(9) atom. There are two inequivalent C sites. In the first C site, C(1) is bonded in a trigonal planar geometry to one O(1), one O(3), and one O(5) atom. In the second C site, C(2) is bonded in a trigonal planar geometry to one O(2), one O(4), and one O(6) atom. There are two inequivalent P sites. In the first P site, P(1) is bonded to one O(11), one O(12), one O(7), and one O(8) atom to form PO4 tetrahedra that share  a cornercorner with one Li(5)O5 trigonal bipyramid. In the second P site, P(2) is bonded to one O(10), one O(13), one O(14), and one O(9) atom to form PO4 tetrahedra that share corners with two equivalent Li(5)O5 trigonal bipyramids. There are fourteen inequivalent O sites. In the first O site, O(1) is bonded to one Li(1), one Li(3), one Li(4), and one C(1) atom to form a mixture of edge and corner-sharing OLi3C tetrahedra. In the second O site, O(2) is bonded to one Na(1), one Li(2), one Li(5), and one C(2) atom to form distorted ONaLi2C tetrahedra that share  a cornercorner with one O(8)Li2MnP trigonal pyramid and  an edgeedge with one O(13)NaLiMnP tetrahedra. In the third O site, O(3) is bonded in a 2-coordinate geometry to one Na(1), one Li(2), one Mn(1), and one C(1) atom. In the fourth O site, O(4) is bonded in a distorted bent 120 degrees geometry to one Li(1), one Mn(2), and one C(2) atom. In the fifth O site, O(5) is bonded in a 5-coordinate geometry to one Li(1), one Li(3), one Li(4), one Mn(1), and one C(1) atom. In the sixth O site, O(6) is bonded in a 1-coordinate geometry to one Na(1), one Li(5), one Mn(2), and one C(2) atom. In the seventh O site, O(7) is bonded in a 4-coordinate geometry to one Na(1), one Li(1), one Mn(1), and one P(1) atom. In the eighth O site, O(8) is bonded to one Li(1), one Li(5), one Mn(1), and one P(1) atom to form distorted OLi2MnP trigonal pyramids that share  a cornercorner with one O(1)Li3C tetrahedra,  a cornercorner with one O(2)NaLi2C tetrahedra,  a cornercorner with one O(13)NaLiMnP tetrahedra, and corners with two equivalent O(11)Li2MnP tetrahedra. In the ninth O site, O(9) is bonded in a 4-coordinate geometry to one Na(1), one Li(2), one Li(3), one Mn(2), and one P(2) atom. In the tenth O site, O(10) is bonded in a 4-coordinate geometry to one Li(2), one Li(4), one Mn(2), and one P(2) atom. In the eleventh O site, O(11) is bonded to one Li(3), one Li(4), one Mn(1), and one P(1) atom to form OLi2MnP tetrahedra that share corners with two equivalent O(8)Li2MnP trigonal pyramids and  an edgeedge with one O(1)Li3C tetrahedra. In the twelfth O site, O(12) is bonded in a 4-coordinate geometry to one Li(3), one Li(4), one Mn(2), and one P(1) atom. In the thirteenth O site, O(13) is bonded to one Na(1), one Li(5), one Mn(2), and one P(2) atom to form distorted ONaLiMnP tetrahedra that share  a cornercorner with one O(8)Li2MnP trigonal pyramid and  an edgeedge with one O(2)NaLi2C tetrahedra. In the fourteenth O site, O(14) is bonded in a distorted rectangular see-saw-like geometry to one Na(1), one Li(5), one Mn(1), and one P(2) atom. is represented by the CIF card [CIF]
data_NaLi5Mn2P2(CO7)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   6.682
_cell_length_b   8.634
_cell_length_c   9.997
_cell_angle_alpha   87.605
_cell_angle_beta   90.000
_cell_angle_gamma   90.000
_symmetry_Int_Tables_number   1
_cell_volume   576.282
_cell_formula_units_Z   2
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Na  Na0  1  0.998  0.248  0.876  1.0
  Na  Na1  1  0.498  0.752  0.124  1.0
  Li  Li2  1  0.255  0.084  0.619  1.0
  Li  Li3  1  0.250  0.091  0.124  1.0
  Li  Li4  1  0.030  0.266  0.368  1.0
  Li  Li5  1  0.468  0.267  0.366  1.0
  Li  Li6  1  0.475  0.270  0.865  1.0
  Li  Li7  1  0.530  0.734  0.632  1.0
  Li  Li8  1  0.968  0.733  0.634  1.0
  Li  Li9  1  0.975  0.730  0.135  1.0
  Li  Li10  1  0.755  0.916  0.381  1.0
  Li  Li11  1  0.750  0.909  0.876  1.0
  Mn  Mn12  1  0.746  0.351  0.633  1.0
  Mn  Mn13  1  0.748  0.354  0.143  1.0
  Mn  Mn14  1  0.246  0.649  0.367  1.0
  Mn  Mn15  1  0.248  0.646  0.857  1.0
  P  P16  1  0.250  0.406  0.602  1.0
  P  P17  1  0.249  0.408  0.109  1.0
  P  P18  1  0.750  0.594  0.398  1.0
  P  P19  1  0.749  0.592  0.891  1.0
  C  C20  1  0.750  0.038  0.614  1.0
  C  C21  1  0.759  0.043  0.112  1.0
  C  C22  1  0.250  0.962  0.386  1.0
  C  C23  1  0.259  0.957  0.888  1.0
  O  O24  1  0.249  0.108  0.415  1.0
  O  O25  1  0.282  0.099  0.923  1.0
  O  O26  1  0.756  0.079  0.737  1.0
  O  O27  1  0.752  0.079  0.237  1.0
  O  O28  1  0.745  0.142  0.516  1.0
  O  O29  1  0.741  0.152  0.019  1.0
  O  O30  1  0.062  0.314  0.649  1.0
  O  O31  1  0.430  0.307  0.656  1.0
  O  O32  1  0.067  0.303  0.151  1.0
  O  O33  1  0.432  0.318  0.168  1.0
  O  O34  1  0.255  0.417  0.445  1.0
  O  O35  1  0.755  0.424  0.350  1.0
  O  O36  1  0.267  0.422  0.953  1.0
  O  O37  1  0.729  0.426  0.840  1.0
  O  O38  1  0.255  0.576  0.650  1.0
  O  O39  1  0.755  0.583  0.555  1.0
  O  O40  1  0.229  0.574  0.160  1.0
  O  O41  1  0.767  0.578  0.047  1.0
  O  O42  1  0.562  0.686  0.351  1.0
  O  O43  1  0.930  0.693  0.344  1.0
  O  O44  1  0.567  0.697  0.849  1.0
  O  O45  1  0.932  0.682  0.832  1.0
  O  O46  1  0.245  0.858  0.484  1.0
  O  O47  1  0.241  0.848  0.981  1.0
  O  O48  1  0.256  0.921  0.263  1.0
  O  O49  1  0.252  0.921  0.763  1.0
  O  O50  1  0.749  0.892  0.585  1.0
  O  O51  1  0.782  0.901  0.077  1.0
[/CIF]
.